19 N95- 31774
REPLACEMENT OF CORROSION PROTECTION CHROMATE PRIMERS AND PAINTS USED IN CRYOGENIC APPLICATIONS ON THE SPACE SHUTII.E WITH WIRE ARC SPRAYED ALUMINUM COATINGS.
R. L. Daniel 1, H. L. Sanders 1, and F. R. Zimmerman 2 1Rocketdyne Division of Rockwell International
Huntsville, AL 35806 2Materiais and Processes Labotat_y National Aeronautics and Space Adminisuatim/MSl_
Marshall Space Flight Center,AL 35812
With the advent of new environmental laws restricting volatile organic compounds and hexavalent chrome emissions, "environmentally safe"thermalspray coatings are being devdo0ed to nWiace the uaditio_ cmosion pmtect_ chromate wimers. A wire arc sprayed aluminum coating is being developed for _ion protection of low pressure liquid hydrogen carrying ducts on the Space Shuttle Main Engine. Currently, this hardwat'e utilizes a chromate primer to provide protection against corrosion pitting and stress corrosion cracking inducedby the cryogenic operating enviromnent. The wire arc sprayed aluminum coating has been found to have good potential to provide corrosion protection for flight hardware in cryogenic applications. The coating development, adhesion test, corrosion test and cryogenic flexibility test remdts will be presented.
Chromate primers ate used to provide corrosion wotection for aerospace hardware in cryogenic applications. One such application is the Low Pressure Fuel Turbopump (LPFTP) Discharge Duct used on the Space Shuttle Main Engine. The LPFTP Discharge Duct carries liquid hydrogen (-423 °F) fuel from the Low-Pressure Fuel Tmbopump discharge to the inlet of the High-_ Fuel Tmbopmnp (see Figth'e 1). The l..Pgl'P Discharge Duct is fabricated from 21-6-9 CRF_ (Ma 8.0 to 10.0, Cr 19.0 to 21.5, Ni 5.5 to 7.5)which isinsulatedwithpol_ foam and then nickel plated.
Pittingcoaoak_ and mess _ crackinghasbeen found on theseducts aftervariousperiodsof service. Chloridecontaminationwas identifiedas theinitiatorofthe cccrmion,althoughtheexactsourceof thechloridesisnot known. Even though 21-6-9 CRES is generally considered conosion resistant, the com_ion problem is accentuated by the crevice corrosion situation crealzd under thefoam insulation (1). To prevent this corrosion, a chromated primer system was qualified and has proven to provide
adequate COtln_ion _ for many yesrs.
Howev_', with increm_ health risk and environmental harm due to hazardous materials, many materiaLs are scheduled to be eliminated in the near future. Among the
materials to be eliminated, due to excess emissions of bexavalent chromium and volatile organic compounds (VOCs), is the chromate prim_ system used on the LPFI'P Discharge Duct. Other organic cmtings have been evaluated forthisapplication with little success, primarily because of difficulty meeting the cryogenic adhesion/flexibility
tjqrlw M Dr/fir
Ftgme 1 The Space Shuale Main Engine s_owi_ the Low Pressure _ Turbopump Discharge Duct.
requirements. Due to the excellentadhesivestrengthand cryoge.nic material properties,a wirearcsprayed (WAS_I) aluminum coating is being developed to replace the chromate primers subjected to cryogenic conditiom on rocket engine components.
Although thermal sprayed corrosion protection coatings have been used extensively to date, none have bern develo[_l for cryogenic applications. The WAS aluminum coating developed meets the stringent adhesion and cryogenic flexibility requireanents of the _ Discharge Duct and the coating offerJ very good corrosion protection for steels md mher conos_ i_me anoyt
This report presents the detailsof thecoating developmentprogram completedincludingthermalsway im'ameterdevelopment,surfacepreparationand optimum coating thickness. Corrosion resistance,cryogenic flexibility and adhesion =st resulm are also presented.
brought to you by CORE View metadata, citation and similar papers at core.ac.uk
provided by NASA Technical Reports Server
IT. Coatinf Develoomem
The ceming development includes material and wocess selection, thermal spray pmmne_ development and hardware process_ developnem.
prncess and Material Selectkm
The wire arc g_rayed aluminum coating was selected based on environmental, cost, availability and performaw_ concen_ Metaliz_ coatings were chosen for their proven COtTCeionWotectkm capabilities (2) and their typically high adhesive strength. These coatings not only act as an effective barrier coat but because they are more anodic than steel (see Table I), they act as a sacrificial anode and give galvanic protection to the substrate.Thus, co_on of the subsW_ will be pre_ even whe_ coating coverage may be incomplete or where the coating may be damaged (3). With the addition of a sealant or _ a thermal sprayed coating has long life and iseasy to clean and maintain. The sealant does not affect the _ _.
The wire arc spray process applies metal coatings using metal feedstock in wire form. Two wires serving as the positive and negative electrodes advance to meet in a location in the atomizing gas. A potential is applied to tbe wires so that an arc is formed at tbe wire intersection causing the wire tips to melt. Atomizing gas flows across the arc zone propelling molten metal droplets to the substrate (see Figure 2). Because of the high temperatures in the arc zone and the superheating of the molten particles,wirearcspraycoatings tend to have excellent adhesion and cohesive strength. Substrate heating however, is significantly lowerthanmost thermal sprayprocessesbecause there is no flame. In addition, wire arc spray systems are light and portable allowing for on-site application or repair of coatings.
Figta_ 2 Schematicof the Bot_ TAFA wire arc spraygun. Aluminum and zinc and their alloys are the most commonly used metals for corrosion wotection coatings. Zinc. however, was not considered due to it's excessive rate of corrosion (4). Aluminum and aluminum alloys were initially selected based on their electro-chemical potential, good material properties at cryogenic temperatures, low weight and availability.
Preliminary screening of aluminum and two alloys, Al 4043 and Al 5356, coatings was performed in an effort to select one coating for further study. The screening tests
consisted of flexibility, adhesion and 30 day salt fog exposure. The best performing coating was selected for further evaluation in cryogenic flexibility, thermal cycle testing and extended salt fog exposm_
The parmneter development wocess concentrated on the setup of five fundamental parameters that are common with most tlgntml spray _ These were:
2) Atomizing Gas 3) Sumdeff Dismce 4)Power Settings 5)Gun and PartMotioa
As with most development programs, it soon became evident that the controllable parameters were not independent of each other. In order to evaluate the affects of parameter changes a"goodness" criteria was developed and used to test each change. This criteria was the coatings performaw,e in a bend test. This test is described in detail in the _xperimental Testing" section later in this paper. The coating passes the test if loss of adhesion or coating cracks do not occur. The test is made more severe by decreasing the bend radius.
Several surface preparation techniques were investigated ranging from grit blasting to a light hand sand. An important factor in the decision was the inspection requirements on the LPFTP Discharge DucL Periodically the duct is taken out of service and the foam and chromate paint is stripped off so the exterior can be inspected for corrosion pitting and cracking using IVc dye peneWanL If the exterior of the duct had been severely roughened, as with grit blasting, the IVc dye penetrant would show many false indications because of its extreane sensitivity. Our testing proved this to be true so grit blasting was ruled out from the start. A variety of handsandingtechniques were tried with different grit sand paper. From these test, a light hand sand with 320 grit A1203 sand paper and acetone final clean gave a good surface for coating adhesion and was smooth enough for IVc dye penetrant inspection.
At the beginning of the study, it was assumed that an inert atomizing gas would perform better because of the less likelihood of oxide formation. This turned out to be a false assumption. A variety of atomizing gasses were tried including; argon, 95% Ar - 5% H2, nitrogen, and air. The different gasses were tested using bend tests to evaluate adhesion and microstructure to determine oxide content and density. Surprisingly using argon, argon-hydrogen and nitrogenas theatomizinggasshowed no decrease in oxide content within the microstructure as compared with using air. Also, using air as the atomizing gas showed a marked increase in bond strength over the other three. This higher bond strength is most noticeable on ferrous substrates, although air seems to generally give higher bond strengths
Table I Relative EMF Potenti_ for Galvmic Cc_rmitm(5)
EMF Potentials Ior Galvanic Corrosion Cathodic Protection
NobleEnd Incone1625 024
(cathode) 21-6-9 CRES 0.14
N/Uicy 2024 -0,ss
AI AlloyTons-50 -0.79
(anode) Aiumlnum -0.80
Base End AI Alloy5052 -0.96
ProtectiveCoating Bimetallic (e.g. ThermalSprayAI Corrosion
com ) l ./
!iiiiiiiiiiiiiiiiiiiiiiiiiiiiiiii iiiiii .... ii!ii iiiiiiiiiiiiiiiiiiiiiiiiiiiiiWii!i!!i!i ii
NoblerMetal: 21-6-9 CRES (LPFTP DischargeDuct)
• Noblermetalprotectedfromcorrosion due to sacrificialanocliccoating.
on mmt metals wla= spraying ahuninum.
Three different standoff distances were evalua_A, being 5 in, 7 in and 10 in. The 5 in and 10 in distances tended to degra_ the _ by inere_sing porosity as compared to 7in. 5 in and 7 in gavesimilar good results in the bend test, but the 10 in distance showed a marked reduction in coating adhesion. A standoff distance of 7 in gave the best overall results.
The settings for the power input to the wire arc gun are controlled by the power supply and the wire feed tale. The desired voltage is dialed in and the power supply will vary the amperageoutputneededto maintain that voltage. As the wire feedgateis in_eas_ the mnperageoutputat the power supply will increase to maintain the set voltage. These pmmneW,rs were not varied much since there is only a nmcow operating range for each l_rticular wire material. The voltage is adjusted by running meequipmentandvarying me voltage until a smooth uniform arc achieved as the wired meet. ff thevoltage isslightly above orbelow the optimum point, the wire will pop and spit. The current is set by increasing the wire feed rate to a point just below the speed whea wire popping occurs. The final parameten are shown in Table II.
Development of gun motion was done to achieve approximately 0.001 in of deposited material per pass. The gun motion was provided by an X-Y manipulator. The submate was held smdomry and the gun passed back and forth in front of it. After each crossing pass the Y axis moved up or down a specified amount to provide full coverage as the manipulator moved up and down the length of the substtate. It was found that a Y-step of 0.35 in after
each X-pass gave a uniform coating with consistent thickness. An X-axis traverse velocity of 15 in/sec was found to deposit approximaCly 0.001 in of material. Hardware Pmcessin_ Devdomnent
Several issues were considered during the hardware process devdopment phase. These include wire arc spraying large parts of complicated geometry's (elbows, bends, etc.), coating inspection and qualification, coating removal, coating repair and inspection after coating removal.
The insulalcd liquid hydrogen carrying ducts were the wimary rocket engine components investigated requiring conoskm protection. Typically these parts have complicated geometry's and are difficult to handle and manipulate. With this in mind, part processing became a major consideration. Two methods for part wocessing were considered; robotics/ automation and wire arc spray "by-hand". Due to the high upfront expense for the required robotics to handle the ducts, spraying by-hand was pursued and will be discussed. To prepare for spraying by-hand, a Taguchi design of experiments was performed to determine the primary wocessing conwol facugs and tolerances. Additional work includes spray by hand on practice ducts anddbow_
Inspection and qualification of the wire arc sprayed aluminum coating will be required after processing flight hardware. Methods condsidered, although the work has not been initiated, is visual, thickness measurement (eddy current,dimensional), tape test, and bend test wimess coupons.
After a period of time, typically part refurbishment is required where by IVc dye penetrant inspection is used to determine the existence of corrosion. The primary issue investigated in this study, involves complete removal of the aluminum coating without surface contamination interfering with the penetrant inspection results. The methods of coating removal investigated were low concentration caustic soda (NaOH, KOH), TURCO-4181 alkaline cleaner (currently used to clean flight hardware) and high pressure water (25,000 to 40,000 psi). In addition to part refurbishment, coating removal is required during hardware change out, such as a fuel flow meter replacemenL In this situation a small portion of the coating will be removed and laterrecoated.
Adhesion, corrosion resistance, cryogenic flexibility, and thermal cycle tests were performed to further evaluate the aluminum coating for use as a corrosion protection coating in cryogenic applications on flight hardware.
Adhesion and Flexibility. The bend and tape tests were used to evaluate the coating flexibility and bond strength. The bend test was done using a 1 in by 6 in by 0.050 in metal strip coated with the material to be tested. The coupon and coating were bent over a known radius while at room temperature. After bending, the coatings were inspected for signs of cracking or loss of coating adhesion. If the coating passed the bend test then a certified adhesive tape was appfied over the coating at the bend area and quickly removed. The coating passed the test if none of the coating material spalled from the substrate. The bend and tape test was made increasingly more severe by decreasing the bend radius.
Initially samples were bent around a 0.5 in mandrel as this was the requirement for coatings on the LPFTP discharge duct. As the testing and development proceeded, the procedure included additional bends around a 0.3 in mandrel and a 180 degree bend applied by severely bending the sample back on itself and pressing it flat.
Cryogenic Flexibility. The cryogenic flexibility of the coating was evaluated by subjecting samples to a bend test in liquid nitrogen. The coated samples were loaded in a "V" block test fixture submerged in liquid nitrogen. The samples were allowed to stabilize at liquid nitrogen temperatures (- 320 °F) and then bent to the radius of the fixture using a mandrel of 2.8 inch in diameter. The mandrel size was determined by examining the bend radii of dents in the LPFTP discharge ducts which were damaged by cryo- pumping and selecting the most severe case (the smallest radii) for testing. After warming the samples to ambient temperature, the coatings were examined for evidence of cracking or loss of adhesion.
Salt Fog Exposure. 4 inx 6 in panels were hand sanded and wire arc sprayed with aluminum. Scribes were placed on each sample penetrating the coating and marring the substrate,allowingforevaluation ofthecathodicprotection capabilitiesfor each materialtested.The sampleswere mounted6 degreesfrom theve_rficaland wereplacedina salt
fog cabinet with a 5% salt solution conforming to ASTM B- 117. The coatings and the subsume of the panels were visually examined after 30, 60, 90 and 120 days of exposure. Coatings were removed from the panels for substrate inspection with a weakcausticsodasolution.
Thermal Cycle. A cold flow thermal cycle test was performed using liquid hydrogen (-423 °F). A 21-6-9 ORES
Figure 3 Cold flow test article during wire arc spray process.
Figure 4. Cold flow test article prior to foam insulation.
test duct was coated with a WAS aluminum coating (Figures 3 - 4) and then insulated with polyurethane foam. Liquid hydrogen was passed through the duct until the duct wall temperature stabilized at approximately (-423 °F). That temperature was held for the desired length of time and then allowed to warm up to ambient temperature. Ten 30 minute steady state cycles were performed and one eight hour steady state cycle was performed. After the testing the insulation was removed and the WAS aluminum coating was examined for cracking or loss of adhesion.
HI. Results and Discussion
Pure aluminum, AI 4043 and A1 5356 aluminum alloys were initially screened in an effort to choose one coating for
further study: Coatings were screened based on their adhesion, flexibility and corrosion resistance capabilities. The coating's adhesion strength was evaluated quantitatively from the pass or fail bend test starting with 0-5 in diameter mandrel and going to a 180 degree bend and tape test. Inall cases the pure aluminum coatings performed the best, followed by the AI 5356 coating and lastly the AI 4043 coating.
Each coaling was also evaluated after 30 days of salt fog exposure. Coated 21-6-9 CRES _ were sc_n"bed_h
the coating to the base metal to evaluate the cathodic
protection provided by each material. After the 30 days of salt fog exposure, the coating and the scribe were visually examined for corrosion. The coating was then removed and the subslrate was examined for signs of corrosion. The pure aluminum and the 5356 alloy showed little coating corrosion product and no substrate _on was apperent. There was significantly mote corrosion Ixodect produced from the 4043 alloy and some rest stains were observed on the substrate.
Based on the results of the screening tests, the pure aluminum was chosen for further evaluation. Additional tests included cryogenic bend, extended salt fog exposure up to 120 days, and a thermal cycle cold flow test.
Micrographs of the aluminum coating (see Figure 5) show the typical splat structure of a wire arc coating. The bond line shows an excellent interface even without a grit blasted surface. The coating also exhibits above average density (greater than 95%) for wire arc and no through
Figure 5 Wire arc sprayed ahuninummicrosu'ucturedeposited on non-grit blast $ubstrate, etched, magnification400x. porosity, although for galvanic corrosion protection, some through porosity is acceptable. Surprisingly, there are few oxide strings between the splat particles even though air is used as the atomizing gas. Overall, a well adhered and dense wire arc spray coating.
The list of the final processing parameters is shown in Table If. Using these parameters, in conjunction with the
Hobart TAFA 8835 Wire Arc Spray System, typical coatings as shown in Figure 5, were repeatably produced.
Table II WAS Aluminum Coat Processing Parameten Wire Material
Substrate Material Surface Preparation Gnu Hardware
Spny Parameters Ionization Gas Gas Spray Pressure Wire Feed Rate Voltage
Amperage Spray Distance Motion
Traverse Speed Up/Down Step
OIT AI (HobartTAFA) 1/16 in Diameter
21-6-9 CITES (Niuvnic 40) Hand Sand 320 Grit A1203
Long Cross Nozzle
Air 3.6 in/see 28 Volts
150 Amps 7in
15 in/see 0.35 in
To prepare for wire arc spraying parts by-hand, a Taguchi design of experiments was performed to determine the primary parameters to control and their corresponding tolerances. The process parameters investigated were gun to part stand-off distance, angle of incidence, gun speed and coating thickness. Coatingadhesion and flexibility wee used to evaluate the coating quality. Evaluation of the data revealed that the coating thickness and gun to pert stand-off distance were the primary parameters contributing
significantly to the quality of the coating. Using this information, representative dtr,t elbows were wire arc sprayed by-hand. Parts were processed with two passes while
maintaining a stand-off distance of 5 inches to 7 inches. Visually, the coaling appeared to be high quality. A tape test on the surface of the part verified good coatingadhesion.
Caustic soda. alkaline cleaner and high pressure water was evaluated as coating removal methods. Samples were IVcdyepeneWantinspectedpriortocoating the samples with aluminum. The coating was removed and the samples again IVc dye penelrant inspected. Methods resulting in no background contamination during the inspection were found acceptable. Both the caustic soda and the alkaline cleaner completely removed the coating efficiently, cleanly and no background contamination was found during penetrant inspection. Since the TURCO 4181 is currently used to clean flight hardware, the high pressure water was not pursued. Howeve_ preliminary investigations showed that high pressure water (25,000 - 40,000 psi) satisfactorily removed the coating without damaging the part.
The experimental results reported are for samples prepared with the developed parameters shown above. The surface was prepared with a 320 grit hand sand and acetone handwipe.
Adhesion and Flexibility. The pure aluminum coating passed all bend and tape test (see Figure 6). The Al 53.56 alloy passed only the tape and bend test around the 0.5 inchmandrel. In general, the thinner coatings proved to have better adhesion and cohesive sn'ength. But the pure aluminum coatings up to 0.010 inch thick were
Figure6 Typical bend test sample coated with wire m'csprayed aluminum(bent around 0.5 inch man&el).
found to pass the all of the bend and tape test, including the 180 degreebe_
Cryogenic Flexibility. Pure aluminum coatings of varied thicknesses, ranging from 0.004 inch to 0.010 inch were prepared for the cryogenic rbend test. All coatings
passed the cryogenic bend test.
Corrosion Resistance. During the initial 30 day test phase, coatings of varied thickness were evaluated. Coating thicknesses of 0.003 inch, 0.007 inch and 0.010 inch were tested. Observations of the test panels after 30 days of expesm'e were:
1. no corrosion of the subslrate
2. aluminum oxide formed covering the WASed aluminum coating
3. the thicker coatings tended to blister and loose adhesion
4. the 0.003 inch and 0.007 inch coatings remained in sati_actm_ condition
Since the life of the coating is directly related to the coating thickness, the 0.007 inch coating, which did not blister or debond, (and was expected to last longer) was chosen for further salt fog testing. Additional panels were prepared and tested for 60, 90 and 120 days. Panels before and after 90 and 120 day salt fog exposure are shown in figures 7-9. As shown, the coating remains intact and there is no corrosion of the subslra_. Some exposed base metal can be seen along the edges of the panels and there are some
blotchy areas where the coating appears to have thinned. The exposed metal area of the panel increased when exposed for 120 days. After removal of the coating, examination of the substmte revealed no corrosion.
Although wire arc spray coatings have been used in the past for numerous corrosion prevention applications, its use in a cryogenic environment has been nonexistent. Rocketdyne's commitment to elimination of hazardous
materials on the SSME and other rocket engine systems presented an excellent application for wire arc sprayed aluminum's use in a liquid hydrogen environment. In developing this alternative process for providing corrosion protection for the SSME, a numl:er of innovations were
Parameters were developed that enabled a dense well adhered wire m'c sprayed aluminum coating to be applied to both flat and cylindrical 21-6-9 substrates. It was fonnd that using air as the atomizing gas at a high pressure (80 psi) gave the best miczosU'ucture and bond strength. Using air as the atomizing gas was shown to give higher bonds suength on ferrous substrates than using an inert gas.
The wire arc sprayed aluminum coating was shown tb survive cryogenic bend tests on a 2.8 in OD mandreL This achievement is significant in the fact _ no other corrosion protection paints, other than the currently used hazardous chromate primer, weze able to survive this test.
It was shown that wire arc sprayed pure aluminum provided better corrosion protection on 21-6-9 than the Al 4043 and AI 4043. The wire arc sprayed aluminum proved that it could provide protection for 21-6-9 in 30, 60, 90, and 120 day salt fog test, a significant achievement for any cathodic protection coating.
It was shown that the coating could be sprayed onto representative SSME duct hardware and there are no apparem significant flight hardware processing issues. A cold flow test specimen was cycled from fiquid hydrogen temperatures
Figure7 Corrosion test panel wire arc slnyed with ahmxinmn (as-sprayed).
Ftsm'e 8 Wire arc sprayedaluminumcoating after90 days salt fog exposure.
Selection: Nonferrous Alloys and Pure Metals, 1979, Pages 204-236.
3. Davision, Ralph M., Debold, Terry, and Johnson, Mark,
"Corrosion of Stainless Steels", ASM Metals Handbook, N'mth Edition, "Col 13, Corrosion, 1987, Pages 547-565.
4. Ishikawa, IC, Seki, NL and Tobe, S., "Application of Thermal Spray Coatings to Prevent Corrosion of Construction in Japan", Proceedings of the 1993 national Thermal Spray Conference, Anaheim, CA, 7-11 June 1993. 5. American Welding Society, Corrosion Test of Hame- Sprayed Coated Steel, 19 Year Report. AWS C2.14-74
Figure9 Wire are sprayedaluminum coating after 120dayssah fog exposure.
to ambient repeatably without any degradation in the coating. In summary, it was shown that wire arc sprayed aluminum can be used to replace environmentally undesirable chromate paints and primers used for com3sion protection of
¢ryogeni¢ hydrogen carrying ducts on the Space Shuttle Main Engine.
The authors would like to acknowledge the work of Yoon Liaw, Phil Krotz and Tim McKechnie for material development and analysis and Jim Bonds for wire arc equipment operation and maintenance. This work was performed under the NASA contact NASS-40000.
1. West, John M., "Basic Corrosion and Oxidation", John Wiley & Sons Press, New York, NY, 1980.
2. Hollingsworth, E. H., and Hunsicker, H. Y., "Corrosion Resistance of Aluminum and Aluminum Alloys", ASM Metals Handbook, Ninth Edition, Vol 2, Properties and